Phase field simulation of the columnar dendritic growth and microsegregation in a binary alloy


 Annis Sullivan
 1 years ago
 Views:
Transcription
1 Vol 17 No 9, September 28 c 28 Chin. Phys. Soc /28/17(9)/ Chinese Physics B and IOP Publishing Ltd Phase field simulation of the columnar dendritic growth and microsegregation in a binary alloy Li JunJie( ), Wang JinCheng( ), and Yang GenCang( ) State Key Laboratory of Solidification Processing, Northwestern Polytechnical University, Xi an 7172, China (Received 23 January 28; revised manuscript received 24 February 28) This paper applies a phase field model for polycrystalline solidification in binary alloys to simulate the formation and growth of the columnar dendritic array under the isothermal and constant cooling conditions. The solidification process and microsegregation in the mushy zone are analysed in detail. It is shown that under the isothermal condition solidification will stop after the formation of the mushy zone, but dendritic coarsening will progress continuously, which results in the decrease of the total interface area. Under the constant cooling condition the mushy zone will solidify and coarsen simultaneously. For the constant cooling solidification, microsegregation predicted by a modified Brody Flemings model is compared with the simulation results. It is found that the Fourier number which characterizes microsegregation is different for regions with different microstructures. Dendritic coarsening and the larger area of interface should account for the enhanced Fourier number in the region with well developed second dendritic arms. Keywords: phase field model, solidification, columnar dendrite, microsegregation PACC: 813F, 6475, 7115Q 1. Introduction The formation of complex solidification patterns is a typical nonequilibrium phenomenon and represents a conceptually simple example of selforganization. Consisting of both the columnar and equiaxed dendrites dendritic structures are prevalent in most cast alloys and play an essential role in determining the final quality of casting products. In addition, microsegregation within dendritic structures also has great influences on the performance of products. Therefore, the descriptions of dendritic structures and microsegregation are key steps towards a complete understanding and controlling of solidification process. Many analytical models of microsegregation have been proposed and extended [1 6] to calculate the chemical inhomogeneity at the scale of dendritic arms, but in all these models some simplifications of dendritic morphology were assumed. In principle, the microsegregation has a close relationship with the microstructure. Yan et al [7] showed that using different geometrical models to approximate the shape of dendrite would give different microsegregation patterns. So the proper description of dendritic morphology is important in modelling microsegregation. The phase field method has been successfully employed as a powerful tool for describing complex solidification structures. [8 11] In the phase field simulation the evolution of the microstructure and concentration field can be explicitly tracked in a physical manner, which results in the convenience to analyse the microsegregation. In this paper a phase field model for polycrystalline solidification is applied to simulate the formation and growth of columnar dendritic array. The concentration distribution within dendritic array is analysed and compared with the classical microsegregation models. 2. Phase field model Based on the work of Kim et al, [12] Kobayashi et al [13] and Gránásy et al, [14] we have developed a phase field model for polycrystalline solidification in binary alloys. [15] Evolution of the phase field, orientation field and concentration field are described by 1 φ M φ t = (ε2 φ) Hh (φ) θ wg (φ) + h (φ)[f L (c L ) f S (c S ) (c L c S )f L c L (c L )], (1) Project supported by the National Natural Science Foundation of China (Grant No 54113) and Doctorate Foundation of Northwestern Polytechnical University, China
2 No. 9 Phase field simulation of the columnar dendritic growth and microsegregation in a binary alloy 3517 [ 1 θ M θ t = H h(φ) θ ], (2) θ c t = [D(φ) c] + [D(φ)h (φ)(c L c S ) φ], (3) where f S (c S ) and f L (c L ) are the free energy densities of the solid and liquid phase respectively, h(φ) = φ 2 (3 2φ), g(φ) = φ 2 (1 φ) 2. The solute diffusivity is defined as D(φ) = D S h(φ)+(1 h(φ))d L, D S and D L are the diffusion coefficient in the solid and liquid respectively. c is determined to be the fractionweighted average value of the solid concentration c S and the liquid concentration c L, c = h(φ)c S + [1 h(φ)]c L. In the interface region the chemical potentials of solid f S c S [c S (x, t)] and liquid f L c L [c L (x, t)] are assumed to be equal. See Ref.[15] for more details about this model. During the phase field calculation, an uniform distributed stochastic noise term (the amplitude is.1) is added at the interface in order to simulate the fluctuations, which results in the well developed secondary arms. 3. Results and discussion Solidification processes of the Ni.396mol%Cu alloy under isothermal and constant cooling conditions are simulated. The material parameters are as follows: diffusion coefficients D S = m 2 /s, D L = m 2 /s, interface energy σ =.35 J/m 2, molar volume V m = m 3 /mol, partition coefficient k=.87, magnitude of anisotropy r =.4, mesh size x = y = m, the computational domain size is 2 2 in terms of grid number. The temperature of the system is assumed to be uniform in both the isothermal and constant cooling conditions. In the former case the temperature is set to be 1576K for all the time, while in the latter case it will decrease from 158 K with a constant cooling rate of 75 K/s. As an initial condition, twenty nuclei are set at the left side of the domain, and they will grow into the undercooled melts Dendritic growth under the isothermal condition The evolution of solidification structure in the isothermal case is shown in Fig.1. The solidification starts at the left side boundary, then the initial grains impinge with each other as they have different crystallographic orientations. The dendrites extend faster into the bulk liquid when their < 1 > crystallographic orientation is perpendicular to the left side boundary, and the growth in other directions is suppressed. Therefore a columnar dendritic structure forms. This selection mechanism in the system with an uniform temperature is not really based on a minimum undercooling criterion, but rather on a minimum travel criterion as pointed out by Rappaz and Gandin. [16] Fig.1. Simulated microstructural during isothermal solidification at 1576 K after: (a) 5 ms, (b) 12.5 ms, (c) 25 ms, and (d) 87.5 ms. Figure 2 illustrates the variation of the average concentrations in the liquid c L and solid c S with x at different times, and the schematic representation of three regions divided according to the change of c L. The values of c L and c S are obtained by averaging the calculated concentrations separately in the liquid and solid along the grid line in y direction. It can be found that, in the region I, the side branches are well developed and the spacing of dendritic arms are relatively small, and the average liquid concentration approximately keeps constant in this region. Here we call this region the mushy zone. In region III, called as liquid zone, there is no solid phase and the average liquid concentration holds the initial value because the so
3 3518 Li JunJie et al Vol. 17 lute diffusion length of dendrites is small. The region II is called as dendritic tip zone, where the value of average liquid concentration gradually changes from the one in mushy zone to that in liquid zone. For the temperature is set to be constant in this case, the solidification in the mushy zone will stop, and the average concentrations of liquid and solid will approximately keep constant as shown in Fig.2(a). Fig.2. (a) Variations of the average concentrations in the liquid c L and solid c S with distance x at different times under isothermal condition, and (b) the schematic representation of three regions divided according to the change of c L. Coarsening of dentritic arm is a surface tension driven phenomenon, during which the secondary dendritic arm spacing and the total surface area will decrease. Under isothermal conditions, although the solidification in the mushy zone stops, the coarsening of dendritic arms progresses after the solidification, which can be reflected by exploring the variation of total surface area (Fig.3) and the distribution of liquid concentration (Fig.4). As shown in Fig.3, after the dendrites reach the right boundary of the system, the solid fraction of the whole system will keep constant, while fraction of total interface will decrease due to the dendritic coarsening. Figure 4(a) is the concentration the histogram for the area that x changes from 3 µm to 4 µm at two different times. The two peaks with increasing levels of concentration correspond to solid and interdendritic liquid. The interdendritic liquid peak contains a spread in composition reflecting the positive and negative curvatures of the interface between the liquid and solid. With the coarsening of dendritic arms the interface curvature will be uniform and the high curvature part will disappear, so the interdendritic liquid concentration will become uniform, which can be reflected by the sharpening of the interdendritic liquid peak (see the enlarged graph in Fig.4(a)) Dendritic growth under the constant cooling condition Fig.3. The fractions of solid and interface against solidification time under isothermal and constant cooling conditions. The microstructure evolution under the constant cooling condition is similar to that under the isothermal condition. However the concentration distribution is quite different as shown in Fig.5. The average concentration of solid varies along the x direction and increases with the time as the temperature decreases continuously. Due to the high diffusivity in the liquid, the average concentration of liquid in the mushy zone approximately keeps uniform, but will increase with time. The increases of average concentrations of liquid
4 No. 9 Phase field simulation of the columnar dendritic growth and microsegregation in a binary alloy 3519 and solid in the mushy zone with time indicate the successive solidification in this region after its formation. This can be also observed from the variation of solid fraction with time in Fig.3. The initial quick raise of the solid fraction curve corresponds to the growth of dendrites into the undercooled liquid, and then the following gentle increase indicates the solidification in the mushy zone, which accompanies with the decrease of interface area arising from the dendritic coarsening. The coarsening can also be found from analysing the concentration histogram for the area that x changes from 3 µm to 4 µm at two different times (Fig.4(b)). Other than the increase of the concentration of solid and interdendritic liquid due to the solidification of the mushy zone, the regularity of Fig.4(b) is similar to that of Fig.4(a). Fig.4. Histograms of the fraction of area vs concentration at different times in the region that x changes from 3 µm to 4 µm, under (a) isothermal condition, (b) constant cooling condition. The insert is an enlarged part of the peak in the liquid phase, the data for the insert in (b) have been shifted for better presentation. Fig.5. Variations of the average concentrations in the liquid and solid with x at different times under constant cooling condition Microsegregation within dendritic array under the constant cooling condition Just as shown in Figs.2 and 5, there is a large liquid concentration variety in the dendritic tip zone, which disobeys the assumption made by most analytical microsegregation models, i.e., complete mixing of liquid. Only after the formation of mushy zone, the liquid concentration can be approximately uniform. In addition, it should be noted that the high initial undercooling and cooling rate in our simulation will lead to nonequilibrium solidification. This will also make the simulation results deviate from analytical microsegregation models. However our analyses indicate that nonequilibrium solidification only happens during the initial stage of dendritic tip growth, but not in the whole process. The evolution of the total undercooling as a function of solid fraction for region A (the area with x changing from 5 µm to 15 µm) and region B (the area with x changing from 5 µm to 65 µm) are shown in Fig.6. It can be seen that at the beginning of solidification there is a high undercooling. So nonequilibrium solidification occurs at this stage. With the progress of solidification the solute constituents are rejected into the liquid phase. When the volume fraction of solid is high, which means that the mushy zone has formed, the undercooling in regions A and B will become very low. So the solidification in the mushy zone is near equilibrium.
5 352 Li JunJie et al Vol. 17 Fig.6. The undercooling evolution as a function of the solid fraction. Based on the above analyses, in order to compare simulation results with analytical microsegregation models, we only study the near equilibrium solidification after the formation of mushy zone under the constant cooling condition. One issue pointed by Giovanola and Kurz [5] should be noted, i.e., in this situation the initial state should be c L = c x at f S = f x (instead of c L = c at f S = in the case of standard microsegregation equation), where the value of c x and f x can be chosen at any time after the complete mixing of liquid. After taking this point into account, the standard Scheil equation, lever rule and Brody Flemings model can be modified as: c L = c x ( 1 fs 1 f x ) k 1, (4) 1 (1 k)f x c L = c x, (5) 1 (1 k)f S [ ] k 1 1 (1 2αk)fS 1 2αk c L = c x, (6) 1 (1 2αk)f x where k is the partition coefficient, α is the Fourier number, which characterizes the solidstate diffusion (so called back diffusion). The derivation of equations (4) (6) is given in the Appendix. Some modifications have been proposed to get more exact solutions [2 4] to the back diffusion problem. What we concerned here is the different extents of back diffusion in regions with different microstructures. So we will take α as a fitting parameter and not use the more sophisticated back diffusion models. [2 4] Microsegregation within regions A and B is invested. The microstructure evolutions in regions A and B are shown in Fig.7. It can be seen that the second dendritic arms are well developed in region B, whereas there are only slick primary arms in region A. Microsegregation forming at the stage of mushy zone solidification is shown in Fig.8. It can be found that the simulation results lie between the Scheil equation and lever rule just as expected, and with properly choosing parameter, α=.257 for region A and α=.685 for region B, the Brody Flemings model can agree well with the simulation results. Compared with region A, the increase of Fourier number for region B means an enhanced back diffusion in this region. The solid diffusion coefficient is the same in the two regions, so the enhanced back diffusion should be attributed to their different microstructures. The coarsening of second dendritic arms in region B leads to an increase of arm spacing. This effect equals to increasing the Fourier number just as pointed by Voller and Beckermann. [6] Furthermore, well developed dendrite arms lead to a larger area of solid/liquid interface per unit volume. The amount of solute transferred by solid diffusion is proportional to the interface area. So the effect of back diffusion is pronounced in region B. Fig.7. Simulated microstructure evolution for region A (a) and region B (b).
6 No. 9 Phase field simulation of the columnar dendritic growth and microsegregation in a binary alloy 3521 (2) equilibrium is maintained at the solid liquid interface, i.e., c i S = kc L, where c i S is the solid concentration at the interface and k is the partition coefficient. Fig.A1. Platelike model of dendritic solidification. The solute balance in the volume element can be written as follows: Fig.8. Liquid concentration profiles as a function of the solid fraction for the solidification of mushy zone. 4. Conclusions Polycrystalline solidifications in Ni.396mol%Cu alloy under isothermal and constant cooling conditions are simulated by using the phase field method. The transition from initial equiaxed grains to the columnar dendritic array based on the minimum travel criterion proposed by Rappaz and Gandin [16] is well reproduced by the phase field simulation. Under the isothermal condition solidification will stop after the formation of the mushy zone, but dendritic coarsening will progress continuously, which results in the decrease of the total interface area. Under the constant cooling condition the mushy zone will solidify and coarsen simultaneously. The simulation results of microsegregation agree with the modified Brody Flemings model. It is also found that the Fourier number which characterizes microsegregation is different for regions with and without well developed second dendritic arms. Dendritic coarsening and the larger area of interface should account for the enhanced Fourier number in the region with well developed second dendritic arms. Appendix We consider a small volume element in the mushy zone and approximate the solidification by the planar geometry as shown in Fig.A1. Microsegregation models base on the following assumptions: (1) diffusion in the liquid is complete, i.e., at any point in time the solute concentration in the liquid phase c L is uniform; XS c S dx + X L c L = Xc, (A1) where c is the initial liquid concentration, X S and X L are the lengths of the solid and liquid portions respectively, and X = X S + X L. Dividing through by X and writing the integral in term of the coordinate ξ = x/x, we find that this equation becomes: fs c S dξ + (1 f S )c L = c. By differentiating with respect to time we obtain fs c S t dξ + kc df S L dt c df S L dt (A2) + (1 f S ) dc L dt =. (A3) In the Scheil model the solid diffusion is neglected, which means c S =, then Eq.(A3) reduces to: t c L (1 k)df S = (1 f S )dc L. (A4) Integrating with the initial condition c L = c x at f S = f x (instead of c L = c at f S = in the case of standard microsegregation equation), we have which results in 1 1 k cl c x dc L c L = fl f x df L f L, (A5) ( ) k 1 1 fs c L = c x. (A6) 1 f x This is the modified Scheil equation, which will reduce to standard form when c x = c and f x =. In the Lever rule the solid diffusion is complete and the solid concentration is uniform, so Eq.(A3) becomes c L (1 k)df S = (1 f S )dc L + kf S dc L. (A7) Integrating with the initial condition c L = c x at f S = f x, we can obtain c L = c 1 (1 k)f x 1 + (1 k)f S, (A8)
7 3522 Li JunJie et al Vol. 17 which will reduce to the standard lever rule when c x = c and f x =. For finiterate diffusion in the solid Voller [4] proposed to set fs c S t dξ = βkf dc L S dt, (A9) where β is the diffusion parameter. When β=2α, α is the Fourier number, Eq.(A3) can be written as: c L (1 k)df S = (1 f S )dc L + 2αkf S dc L. (A1) Integrating with the initial condition c L = c x at f S = f x, we get in following result [ ] k 1 1 (1 2αk)fS 1 2αk c L = c x. 1 (1 2αk)f x (A11) In the limit of c x = c and f x =, the standard Brody Flemings equation c L = c [1 f S (1 2αk)] k 1 1 2αk (A12) follows immediately from Eq.(A11). It can be seen that the modified Brody Flemings equation (A11) will reduce to the modified Scheil equation (A6) with α =, and reduce to the modified lever rule (A8) with α =.5. References [1] Brody H D and Flemings M C 1966 Trans. Metall. Soc. AIME [2] Clyne T W and Kurz W 1981 Metall. Trans. A [3] Ohnaka I 1986 Trans. ISIJ [4] Voller V R 1999 J. Crystal Growth [5] Giovanola B and Kurz W 199 Metall. Trans. A [6] Voller V R and Beckermann C 1999 Metall. Mater. Trans. A [7] Yan X, Xie F, Chu M and Chang Y A 21 Mater. Sci. Eng. A [8] Warren J A and Boettinger W J 1995 Acta Metall. Mater [9] Long W Y, Cai Q Z, Wei B K and Chen L L 26 Acta Phys. Sin (in Chinese) [1] Li M E, Xiao Z Y, Yang G C and Zhou Y H 26 Chin. Phys [11] Li J J, Wang J C, Xu Q and Yang G C 27 Acta Phys. Sin (in Chinese) [12] Kim S G, Kim W T and Suzuki T 1999 Phys. Rev. E [13] Kobayashi R, Warren J A and Carter W C 2 Physica D [14] Gránásy L, Pusztai T and Warren J A 24 J. Phys. Condens. Matter [15] Li J J, Wang J C, Xu Q and Yang G C 27 Acta Mater [16] Rappaz M and Gandin Ch A 1993 Acta Metall. Mater
Numerical Simulation of Dendrite Growth during Solidification
Freund Publishing House Ltd. International Journal of Nonlinear Sciences and Numerical Simulation, 7(2), 171176, 2006 Numerical Simulation of Dendrite Growth during Solidification X. Yao a b, B. He b,
More informationModification of Ohnaka back diffusion equation
IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS Modification of Ohnaka back diffusion equation To cite this article: A Turkeli 2016 IOP Conf. Ser.: Mater. Sci. Eng. 117 012021
More informationEvolution of the Specific SolidLiquid Interface Area in Directional Solidification
Evolution of the Specific SolidLiquid Interface Area in Directional Solidification Beckermann C 1), NeumannHeyme H 2), Eckert K 2) 1 Department of Mechanical and Industrial Engineering, University of
More informationNumerical Simulation of Solidification Structure Formation during Continuous Casting in Fe 0.7mass%C Alloy Using Cellular Automaton Method
, pp. 903 908 Numerical Simulation of Solidification Structure Formation during Continuous Casting in Fe 0.7mass%C Alloy Using Cellular Automaton Method Minoru YAMAZAKI, 1) Yukinobu NATSUME, 1) Hiroshi
More information1. Introduction. Alexandre Furtado Ferreira a *, Ivaldo Leão Ferreira a, Janaan Pereira da Cunha a, Ingrid Meirelles Salvino a
Materials Research. 2015; 18(3): 644653 2015 DOI: http://dx.doi.org/10.1590/15161439.293514 Simulation of the Microstructural Evolution of Pure Material and Alloys in an Undercooled Melts via Phasefield
More informationAnalysis of Yield Rate in Single Crystal Casting Process Using an Engineering Simulation Model
Materials Transactions, Vol. 44, No. 5 (23) pp. 829 to 835 Special Issue on Solidification Science and Processing for Advanced Materials #23 The Japan Institute of Metals Analysis of Yield Rate in Single
More informationPhase Transformation in Materials
2015 Fall Phase Transformation in Materials 11. 11. 2015 Eun Soo Park Office: 33313 Telephone: 8807221 Email: espark@snu.ac.kr Office hours: by an appointment 1 Contents for previous class Solidification:
More informationSegregation and Microstructure in Continuous Casting Shell
Segregation and Microstructure in Continuous Casting Shell Brian G. Thomas and YoungMok Won Department of Mechanical & Industrial Engineering University of Illinois at UrbanaChampaign September 25, 2000
More informationPhasefield Model for Solidification of Ternary Alloys
, pp. 870 876 Phasefield Model for Solidification of Ternary Alloys Machiko ODE, Jae Sang LEE, 1 Seong Gyoon KIM, Won Tae KIM 3 and Toshio SUZUKI 4 Graduate School, The University of Tokyo, Tokyo 1138656
More informationA TwoDimensional Computational Model for the Simulation of Dendritic Microstructure and Solute Distribution of Fe0.04%C Alloys
World Journal of Engineering and Technology, 2017, 5, 175187 http://www.scirp.org/journal/wjet ISSN Online: 23314249 ISSN Print: 23314222 A TwoDimensional Computational Model for the Simulation of
More informationSimulation of Solute Redistribution during Casting and Solutionizing of Multiphase, Multicomponent Aluminum Alloys
Simulation of Solute Redistribution during Casting and Solutionizing of Multiphase, Multicomponent Aluminum Alloys F. Yi,* H. D. Brody* and J. E. Morral** * University of Connecticut, Storrs, CT 6269336
More informationStatic Recrystallization PhaseField Simulation Coupled with Crystal Plasticity Finite Element Method
tatic Recrystallization PhaseField imulation Coupled with Crystal Plasticity Finite Element Method T. Takaki 1, A. Yamanaka, Y. Tomita 2 ummary We have proposed a simulation model for static recrystallization
More informationSimple Model of Microsegregation. during Solidification of Steels REPORT. YoungMok Won Brian G. Thomas. Continuous Casting Consortium
Metal Process Simulation Laboratory Department of Mechanical and Industrial Engineering University of Illinois at UrbanaChampaign Urbana, IL 61801 Simple Model of Microsegregation during Solidification
More informationK S T S ' = K L T L ' + vl v
Heat Flow and Interface Stability Elemental metals  solidification rate controlled by rate at which latent of fusion can be conducted away from the solid/liquid interface Heat conduction can be either
More informationSolidification microstructure development
Sadhana, Vol. 6, Parts 1 &, February April 001, pp. 5 34. Printed in India Solidification microstructure development G PHANIKUMAR and K CHATTOPADHYAY Department of Metallurgy, Indian Institute of Science,
More informationModeling of Globular and Dendritic Structure Evolution in Solidification of an Al 7mass%Si Alloy
, pp. 99 998 Modeling of Globular and Dendritic Structure Evolution in Solidification of an Al 7mass%Si Alloy M. F. ZHU, J. M. KIM and C. P. HONG Center for ComputerAided Materials Processing (CAMP),
More informationThe accuracy of a 2D and 3D dendritic tip scaling parameter in predicting the columnar to equiaxed transition (CET)
Journal of Physics: Conference Series PAPER OPEN ACCESS The accuracy of a 2D and 3D dendritic tip scaling parameter in predicting the columnar to equiaxed transition (CET) To cite this article: M Seredyski
More informationMACRO AND MICROSTRUCTURES
CHAPTER 11 MACRO AND MICROSTRUCTURES Movies from simulations relating to macromicro models of solidification can be found at: http://solidification.org/movies/macromicro. html 11.1 INTRODUCTION The
More informationPHYSICAL AND MATHEMATICAL MODELLING OF THE INITIAL SHELL STRENGTH IN CONTINUOUS CASTING
PHYSICAL AND MATHEMATICAL MODELLING OF THE INITIAL SHELL STRENGTH IN CONTINUOUS CASTING Schuetzenhoefer, W., C. Bernhard and H. Hiebler Department of Ferrous Metallurgy, University of Leoben, Austria ABSTRACT
More informationFractal characteristics of dendrite in aluminum alloys
IOP Conference Series: Materials Science and Engineering Fractal characteristics of dendrite in aluminum alloys To cite this article: K Ohsasa et al 2012 IOP Conf. Ser.: Mater. Sci. Eng. 33 012108 View
More informationInfluence of directional solidification variables on primary dendrite arm spacing of Nibased superalloy DZ125
Influence of directional solidification variables on primary dendrite arm spacing of Nibased superalloy DZ125 *Zhang Weiguo, Liu Lin, Huang Taiwen, Zhao Xinbao, Qu Min, Yu Zhuhuan, Fu Hengzhi (State Key
More informationSolidification Path and Solute Redistribution of an IronBased MultiComponent Alloy with Solute Diffusion in the Solid
Materials Transactions, Vol. 43, No. 11 (22) pp. 289 to 2896 c 22 The Japan Institute of Metals olidification Path and olute Redistribution of an IronBased MultiComponent Alloy with olute Diffusion in
More informationLecture 31: Principles of Solidification of Steel. Key words: Solidification, planar growth, dendritic growth, casting, constitutional supercooling
Lecture 31: Principles of Solidification of Steel Contents: Preamble Solidification variables Equilibrium solidification Non equilibrium solidification Microstructure development Key words: Solidification,
More informationThe peritectic transformation, where δ (ferrite) and L (liquid)
Cellular automaton simulation of peritectic solidification of a CMn steel *Su Bin, Han Zhiqiang, and Liu Baicheng (Key Laboratory for Advanced Materials Processing Technology (Ministry of Education),
More informationLecture 6: Solidification of Single Phase Alloys
Lecture 6: Solidification of Single Phase Alloys 1 Zone Melting Process of zone melting: Start with a solid alloy bar with uniform crosssection. Place the bar horizontally. Only melt the bar within a
More informationModeling of microstructure evolution of magnesium alloy during the high pressure die casting process
IOP Conference Series: Materials Science and Engineering Modeling of microstructure evolution of magnesium alloy during the high pressure die casting process To cite this article: Mengwu Wu and Shoumei
More informationSIMULATION OF DIFFUSIONAL PROCESSES DURING SOLIDIFICATION IN AUSTENITIC STEELS
Abstract SIMULATION OF DIFFUSIONAL PROCESSES DURING SOLIDIFICATION IN AUSTENITIC STEELS D. Baldissin*, L. Battezzati, Dipartimento di Chimica IFM e Centro di Eccellenza NIS, Università di Torino, Via P.
More informationModeling Macrosegregation with a Multiphase Approach: Examples and Discussions
Modeling Macrosegregation with a Multiphase Approach: Examples and Discussions Menghuai Wu and Andreas Ludwig Simulation and Modeling of Metallurgical Processes, Department of Metallurgy, University of
More informationPredicting SecondaryDendrite Arm Spacing of the Al4.5wt%Cu Alloy During Unidirectional Solidification
Materials Research. DOI: http://dx.doi.org/10.1590/19805373mr20150150 Predicting SecondaryDendrite Arm Spacing of the Al4.5wt%Cu Alloy During Unidirectional Solidification Alexandre Furtado Ferreira
More informationEvaluation of dendrite morphology using fractal dimension and dimensionless perimeter in unidirectionally solidified AlSi Alloys
IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS Evaluation of dendrite morphology using fractal dimension and dimensionless perimeter in unidirectionally solidified AlSi Alloys
More informationV. R. Voller University of Minnesota
Micromacro Modeling of Solidification Processes and Phenomena, in Computational Modeling of Materials, Minerals and Metals Processing (eds M. Cross, J.W. Evans, and C. Bailey), TMS Warrendale, 2001. V.
More informationSolidification. Nov. 2010
Solidification Nov. 2010 Rapid Solidification (10 5 K/s) Rapidly cool or quench to produce amorphous or glassy structure (metallic glass) Rapid Solidification Cooling
More informationModeling: (i) thermal spray rapid solidification (ii) partially molten particle impact
Modeling: (i) thermal spray rapid solidification (ii) partially molten particle impact Markus Bussmann Mechanical & Industrial Engineering Centre for Advanced Coating Technologies (CACT) University of
More informationNumerical modelling of the solidification of ductile iron
Journal of Crystal Growth 191 (1998) 261 267 Numerical modelling of the solidification of ductile iron J. Liu*, R. Elliott Manchester Materials Science Centre, University of Manchester, Grosvenor Street,
More informationModule 22. Solidification & Binary Phase Diagrams V. Lecture 22. Solidification & Binary Phase Diagrams V
Module 22 Solidification & Binary Phase Diagrams V ecture 22 Solidification & Binary Phase Diagrams V 1 NPTE Phase II : IIT Kharagpur : Prof. R. N. Ghosh, Dept of Metallurgical and Materials Engineering
More informationThermoCalc Application for the Assessment of Binary Alloys NonEquilibrium Solidification
A R C H I V E S of F O U N D R Y E N G I N E E R I N G Published quarterly as the organ of the Foundry Commission of the Polish Academy of Sciences ISSN (1897331) Volume 17 Issue 1/217 163 168 3/1 ThermoCalc
More informationMICROSTRUCTURE OF RAPIDLY SOLIDIFIED POWDERS
MICROSTRUCTURE OF RAPIDLY SOLIDIFIED POWDERS R. D. Field, A. R. Cox,J"' and H. L. Fraser?+ Department of Metallurgical and Mining Engineering University of Illinois Urbana, Illinois 61801 Individual rapidly
More informationDetermination of the cast structure parameter on the basis of microsegregation analysis
Determination of the cast structure parameter on the basis of microsegregation analysis J. Dobrovská 1, F. Kavička 2, K. Stránský 2 and V. Dobrovská 1 1 Faculty of Metallurgy and Materials Engineering,
More informationPhasefield simulation of the columnartoequiaxed transition in alloy solidification
Acta Materialia 54 (26) 215 226 www.actamatjournals.com Phasefield simulation of the columnartoequiaxed transition in alloy solidification Arnoldo Badillo, Christoph Beckermann * Department of Mechanical
More informationA Phase Field Model for Grain Growth and Thermal Grooving in Thin Films with Orientation Dependent Surface Energy
Solid State Phenomena Vol. 129 (2007) pp. 8994 online at http://www.scientific.net (2007) Trans Tech Publications, Switzerland A Phase Field Model for Grain Growth and Thermal Grooving in Thin Films with
More informationNumerical Simulation of the Solidification of Pure Melt by a Phase Field Model Using an Adaptive Computation Domain
Numerical Simulation of the Solidification of Pure Melt by a PhaseField Model Using an Adaptive Computation Domain Alexandre Furtado Ferreira furtado@metal.eeimvr.uff.br Universidade Federal Fluminense
More informationCFD MODELLING OF MACROSEGREGATION AND SHRINKAGE IN LARGE DIAMETER STEEL ROLL CASTINGS: A COMPARISON ON SEN AND DLP TECHNIQUES
Ninth International Conference on CFD in the Minerals and Process Industries CSIRO, Melbourne, Australia 1012 December 2012 CFD MODELLING OF MACROSEGREGATION AND SHRINKAGE IN LARGE DIAMETER STEEL ROLL
More informationA molecular dynamics study on melting point and specific heat of Ni 3 Al alloy
Science in China Series G: Physics, Mechanics & Astronomy 2007 SCIENCE IN CHINA PRESS Springer A molecular dynamics study on melting point and specific heat of Ni 3 Al alloy YANG Hong, LÜ YongJun, CHEN
More informationModeling of FerriteAustenite Phase Transformation Using a Cellular Automaton Model
, pp. 422 429 Modeling of FerriteAustenite Phase Transformation Using a Cellular Automaton Model Dong AN, 1) Shiyan PAN, 1) Li HUANG, 1) Ting DAI, 1) Bruce KRAKAUER 2) and Mingfang ZHU 1) * 1) Jiangsu
More informationMultiscale simulation of ductile iron casting
IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS Multiscale simulation of ductile iron casting To cite this article: J Kubo 2015 IOP Conf. Ser.: Mater. Sci. Eng. 84 012044 View
More informationTHE INFLUENCE OF Nb AND C ON THE SOLIDIFICATION MICROSTRUCTURES OF FeNiCr ALLOYS
Pergamon Scripta Materialia, Vol. 41, No. 4, pp. 449 454, 1999 Elsevier Science Ltd Copyright 1999 Acta Metallurgica Inc. Printed in the USA. All rights reserved. 13596462/99/$ see front matter PII S13596462(99)001025
More informationA Simple Model to Calculate Dendrite Growth Rate during Steel Continuous Casting Process
, pp. 1792 1796 A Simple Model to Calculate Dendrite Growth Rate during Steel Continuous Casting Process Mujun LONG, 1) Lifeng ZHANG, 2) and Fei LU 3) 1) Visiting Scholar at Department of Materials Science
More informationGRAIN GROWTH MODELING FOR ADDITIVE MANUFACTURING OF NICKEL BASED SUPERALLOYS
Proceedings of the 6th International Conference on Recrystallization and Grain Growth (ReX&GG 016) Edited by: Elizabeth A. Holm, Susan Farjami, Priyadarshan Manohar, Gregory S. Rohrer, Anthony D. Rollett,
More informationEquiaxed and columnar dendrite growth simulation in Al7Si Mg ternary alloys using cellular automaton method
IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS Equiaxed and columnar dendrite growth simulation in Al7Si Mg ternary alloys using cellular automaton method To cite this article:
More informationA Solidification Model for Atomization
, pp. 992 999 A Solidification Model for Atomization Arvind PRASAD, 1) Salem MOSBAH, 2) Hani HENEIN 1) and CharlesAndré GANDIN 2) 1) Department of Chemical and Materials Engineering, University of Alberta,
More informationPreCourse Reading for ESI s Solidification Course
PreCourse Reading for ESI s Solidification Course A. B. Phillion, J. Dantzig The primary goal of ESI s Solidification Course is to relate material properties and solidification processing conditions to
More informationModeling of solutal dendritic growth with melt convection
Computers and Mathematics with Applications 55 (2008) 1620 1628 www.elsevier.com/locate/camwa Modeling of solutal dendritic growth with melt convection MingFang Zhu a,, Ting Dai a, SungYoon Lee b, ChunPyo
More informationGrowth of equiaxed dendritic crystals settling in an undercooled melt
Growth of equiaxed dendritic crystals settling in an undercooled melt A. Badillo and C. Beckermann Dept. Mechanical & Industrial Engineering, University of Iowa, SC, Iowa City, IA, USA Abstract Experiments
More informationBuilding blocks for a digital twin of additive manufacturing
Building blocks for a digital twin of additive manufacturing  a path to understand the most important metallurgical variables H.L. Wei, T. Mukherjee and T. DebRoy, Department of Materials Science and
More informationEffect of Iron Content on Hot Tearing of HighStrength AlMgSi Alloy
Materials Transactions, Vol. 47, No. () pp. 8 to 87 # The Japan Institute of Metals Effect of Iron Content on Hot Tearing of HighStrength AlMgSi Alloy Hiromi Nagaumi, Satoru Suzuki, Toshimitsu Okane
More informationMicroSegregation along the Monovariant Line in a Ternary Eutectic Alloy System
Materials Transactions, Vol. 44, No. 5 (23) pp. 8 to 88 Special Issue on Solidification Science Processing for Advanced Materials #23 The Japan Institute of Metals MicroSegregation along the Monovariant
More informationMathematical Modeling of Solidification Paths in Ternary Alloys: Limiting Cases of Solute Redistribution
Mathematical Modeling of Solidification Paths in Ternary Alloys: Limiting Cases of Solute Redistribution J.N. DuPONT Asimple mathematical framework is provided for calculating solidification paths of ternary
More informationThe effect of alloy elements on the density variation of steel melt at the interdendritic region during solidification
IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS The effect of alloy elements on the density variation of steel melt at the interdendritic region during solidification To cite
More informationPhase Field Modeling of the Effects of Gradient Energy Coefficients on. the Voidmatrix Interface Thickness during Czochralski Silicon Crystal
International Conference on Manufacturing Science and Engineering (ICMSE 2015) Phase Field Modeling of the Effects of Gradient Energy Coefficients on the Voidmatrix Interface Thickness during Czochralski
More informationProgress on modeling and simulation of directional solidification of superalloy turbine blade casting. *Xu Qingyan, Liu Baicheng, Pan Dong, Yu Jing
Progress on modeling and simulation of directional solidification of superalloy turbine blade casting *Xu Qingyan, Liu Baicheng, Pan Dong, Yu Jing (Key Laboratory for Advanced Materials Processing Technology,
More informationSEGREGATION DURING SOLIDIFICATION
SEGREGATION DURING SOLIDIFICATION IN THE MARM247 SYSTEM K.L. ZeislerMash1 and B.J. Pletka Department of Metallurgical and Materials Engineering Michigan Technological University Houghton, Michigan 49931
More informationMODELLING OF THE THERMOPHYSICAL AND PHYSICAL PROPERTIES FOR SOLIDIFICATION OF ALALLOYS
Light Metals 23 Edited by P. Crepeau (Warrendale, PA: TMS, 23), 999. MODELLING OF THE THERMOPHYSICAL AND PHYSICAL PROPERTIES FOR SOLIDIFICATION OF ALALLOYS N.Saunders 1, X.Li 2, A.P.Miodownik 1 and J.P.Schillé
More informationHotcrack test for aluminium alloys welds using TIG process
EPJ Web of Conferences 6, 07001 (2010) DOI:10.1051/epjconf/20100607001 Owned by the authors, published by EDP Sciences, 2010 Hotcrack test for aluminium alloys welds using TIG process A. Niel,a, F. Deschauxbeaume,
More informationThermodynamics and Microstructure: Recent Examples for Coupling of Thermodynamic and Mobility Data to the Software MICRESS
12.09.08 Aachen Thermodynamics and Microstructure: Recent Examples for Coupling of Thermodynamic and Mobility Data to the Software MICRESS Dr. Bernd Böttger ACCESS e.v. Aachen Outline Microstructure Simulation
More informationAnalysis of Crack Susceptibility of Regular Carbon Steel Slabs Using VolumeBased Shrinkage Index
, pp. 1812 1817 Analysis of Crack Susceptibility of Regular Carbon Steel Slabs Using VolumeBased Shrinkage Index Jianfei XU, 1) Shengping HE, 1) * Xueping JIANG, 2) Ting WU 1) and Qian WANG 1) 1) College
More informationNumerical Simulation of Microstructure Evolution of Al Alloys in Centrifugal Casting
, pp. 738 747 Numerical Simulation of Microstructure Evolution of Al Alloys in Centrifugal Casting S. R. CHANG, J. M. KIM and C. P. HONG Center for ComputerAided Materials Processing (CAMP), Department
More informationDescription of the Hypoperitectic Steel Solidification under Continuous Cooling and Crack Susceptibility
, pp. 454 460 Description of the Hypoperitectic Steel Solidification under Continuous Cooling and Crack Susceptibility José Jorge RUÍZ MONDRAGÓN, 1) Martín HERRERA TREJO, 1) Manuel de JESÚS CASTRO ROMÁN
More informationModes of Grain Selection in Spiral Selector during Directional Solidification of Nickelbase Superalloys
J. Mater. Sci. Technol., 12, 28(3), 214 2. Modes of Grain Selection in Spiral Selector during Directional Solidification of Nickelbase Superalloys Xiangbin Meng 1,2), Qi Lu 1,2), Jinguo Li 1), Tao Jin
More informationANALYSIS AND INTERPRETATION OF MAXUS7 EXPERIMENTS MACE ON COLUMNAREQUIAXED SOLIDIFICATION IN ALSI ALLOYS
ANALYSIS AND INTERPRETATION OF MAXUS7 EXPERIMENTS MACE ON COLUMNAREQUIAXED SOLIDIFICATION IN ALSI ALLOYS Laszlo Sturz, Gerhard Zimmermann ACCESS e.v., Intzestrasse 5, 52072 Aachen, Germany, Email: L.Sturz@accesstechnology.de
More informationPhysical Metallurgy Friday, January 28, 2011; 8:30 12:00 h
Physical Metallurgy Friday, January 28, 2011; 8:30 12:00 h Always motivate your answers All subquestions have equal weight in the assessment Question 1 Precipitationhardening aluminium alloys are, after
More informationGrain Morphology of AsCast Wrought Aluminium Alloys
Proceedings of the 12th International Conference on Aluminium Alloys, September 59, 2010, Yokohama, Japan 2010 2010 The Japan Institute of Light Metals pp. 173178 173 Grain Morphology of AsCast Wrought
More informationProbabilistic Simulation of Solidification Microstructure Evolution During LaserBased Metal Deposition
Probabilistic Simulation of Solidification Microstructure Evolution During LaserBased Metal Deposition Jingwei Zhang1, Frank Liou1, William Seufzer3, Joseph Newkirk2, Zhiqiang Fan1, Heng Liu1, Todd E.Sparks1
More information3rd International Conference on Mechatronics and Information Technology (ICMIT 2016)
3rd International Conference on Mechatronics and Information Technology (ICMIT 2016) The confirmation of simulation parameter and analysis of temperature field of 430 ferrite stainless steel in watercooling
More informationExperimentallyaided Simulation of Directional Solidification of Steel
, pp. 526 532 Experimentallyaided Simulation of Directional Solidification of Steel Salar NIKNAFS* and Rian DIPPENAAR University of Wollongong, Northfields Avenue, Gwynneville, NSW 2500, Australia. (Received
More informationFinite Element Simulation of the Process of Aluminum. Alloy Resistance Spot Welding
Finite Element Simulation of the Process of Aluminum Alloy Resistance Spot Welding Li Baoqing, Shan Ping, Lian Jinrui, Hu Shengsun, Cheng Fangjie Tianjin University, Tianjin, P.R.C Abstract In this paper,
More informationPartial melting and resolidification in partially melted zone during gas tungsten arc welding of AZ91 cast alloy
Partial melting and resolidification in partially melted zone during gas tungsten arc welding of AZ91 cast alloy T. P. ZHU 1, Z. W. CHEN 2, W. GAO 1 1. Department of Chemical and Materials Engineering,
More informationMODELLING OF THE THERMOPHYSICAL AND PHYSICAL PROPERTIES FOR SOLIDIFICATION OF ALALLOYS
Light Metals 23 Edited by P. Crepeau TMS (The Minerals, Metals & Materials Society), 23 MODELLING OF THE THERMOPHYSICAL AND PHYSICAL PROPERTIES FOR SOLIDIFICATION OF ALALLOYS N.Saunders 1, X.Li 2, A.P.Miodownik
More informationDIRECTIONAL SOLIDIFICATION OF CMSX3 NICKEL BASED SUPERALLOY
DIRECTIONAL SOLIDIFICATION OF CMSX3 NICKEL BASED SUPERALLOY Peter PINKE Maroš MARTINKOVIČ Faculty of Materials Science and Technology Trnava, Slovak University of Technology Bratislava, Paulínska 16,
More informationmodeling of grain growth and coarsening in multicomponent alloys
Quantitative phasefield modeling of grain growth and coarsening in multicomponent alloys N. Moelans (1) Department of metallurgy and materials engineering, K.U.Leuven, Belgium (2) Condensed Matter &
More informationCast Alloys for Advanced Ultra Supercritical Steam Turbines. Gordon R. Holcomb, Ping Wang, Paul D. Jablonski, and Jeffrey A. Hawk
Cast Alloys for Advanced Ultra Supercritical Steam Turbines Gordon R. Holcomb, Ping Wang, Paul D. Jablonski, and Jeffrey A. Hawk Surface Stability of Materials in HighTemperature Aggressive Environments,
More informationSolidification: basics and beyond Equilibrium and nonequilibrium solidification
Solidification: basics and beyond Equilibrium and nonequilibrium solidification Prof. Dmitry Eskin BCAST NETCENG, 2015 1 Types of solidification reactions Equilibrium solidification 2 Gibbs phase rule
More informationTALAT Lecture Phase Diagrams. 14 pages, 13 Figures. Basic Level
TALAT Lecture 1203 Phase Diagrams 14 pages, 13 Figures Basic Level prepared by M H Jacobs * Interdisciplinary Research Centre in Materials The University of Birmingham, UK (Based on approach adopted by
More informationManifoldvalued equation with singular diffusivity
1441 2005 3237 32 Mathematical model of the evolution of polycrystalline structures  Manifoldvalued equation with singular diffusivity Ryo Kobayashi 1, James A. Warren 2 1 Department of Mathematical
More informationSolidification & Binary Phase Diagrams II. Solidification & Binary Phase Diagrams II
Module 19 Solidification & inary Phase Diagrams II ecture 19 Solidification & inary Phase Diagrams II 1 NPTE Phase II : IIT Kharagpur : Prof. R. N. hosh, Dept of Metallurgical and Materials Engineering
More informationSynchrotron Xray Imaging and Numerical Modelling of Dendritic Sidebranch Evolution during Coarsening
Synchrotron Xray Imaging and Numerical Modelling of Dendritic Sidebranch Evolution during Coarsening H. NeumannHeyme 1, N. Shevchenko 1, K. Eckert 1,2, J. Grenzer 1, C. Beckermann 3 and S. Eckert 1 1
More informationSolidification and Crystallisation 5. Formation of and control of granular structure
MME 345 Lecture 08 Solidification and Crystallisation 5. Formation of and control of granular structure Ref: [1] A. Ohno, The Solidification of Metals, Chijin Shokan Co. Ltd., 1976 [2] P. Beeley, Foundry
More informationmodeling of grain growth and coarsening in multicomponent alloys
Quantitative phasefield modeling of grain growth and coarsening in multicomponent alloys N. Moelans (1), L. Vanherpe (2), A. Serbruyns (1) (1), B. B. Rodiers (3) (1) Department of metallurgy and materials
More informationMODELLING OF EQUIAXED GRAIN GROWTH IN SOLIDIFICATION PROCESS
76/14 Archives of Foundry, Year 004, Volume 4, 14 Archiwum Odlewnictwa, Rok 004, Rocznik 4, Nr 14 PAN Katowice PL ISSN 1645308 MODELLING OF EQUIAXED GRAIN GROWTH IN SOLIDIFICATION PROCESS O. WODO 1, N.
More informationComputer simulation of grain growth kinetics with solute drag
Journal of MATERIALS RESEARCH Welcome Comments Help Computer simulation of grain growth kinetics with solute drag D. Fan P.O. Box 5800, MS 1411, Sandia National Laboratories, Albuquerque, New Mexico 87185
More informationSolidification of NbBearing Superalloys: Part II. Pseudoternary Solidification Surfaces
Solidification of NbBearing Superalloys: Part II. Pseudoternary Solidification Surfaces J.N. DuPONT, C.V. ROBINO, A.R. MARDER, and M.R. NOTIS Equilibrium distribution coefficients and pseudoternary solidification
More informationAnomalous Halo Formation in an ArcMelted ScNiSc 2 Ni OffEutectic Binary Alloy
materials Communication Anomalous Halo Formation in an ArcMelted ScNiSc 2 Ni OffEutectic Binary Alloy Kai Wang, Ming Wei and Lijun Zhang * State Key Laboratory of Powder Metallugy, Central South University,
More informationAN IMPROVED RAYLEIGH NUMBER CRITERION FOR FRECKLE PREDICTION INCORPORATING THE EFFECT OF CARBIDES
AN IMPROVED RAYLEIGH NUMBER CRITERION FOR FRECKLE PREDICTION INCORPORATING THE EFFECT OF CARBIDES Y.M. Youssef 1, D. Ness 1, E. Cutler 2, G.E. Fuchs 2 and P.D. Lee 1* 1 Department of Materials, Imperial
More informationThe Effects of Superheating Treatment on Distribution of Eutectic Silicon Particles in A357Continuous Stainless Steel Composite.
Please cite this paper as M. N. Mazlee & J. B. Shamsul. (2012). The Effects of Superheating Treatment on Distribution of Eutectic Silicon Particles in A357Continuous Stainless Steel Composite, Advanced
More informationSimple Model of Microsegregation during Solidification of Steels
Simple Model of Microsegregation during Solidification of Steels YOUNGMOK WON and BRIAN G. THOMAS A simple analytical model of microsegregation for the solidification of multicomponent steel alloys is
More informationEffect of Al5Ti1B master alloy on microstructures and properties of AZ61 alloys
Effect of Al5Ti1B master alloy on microstructures and properties of AZ61 alloys MA Xuliang( ) 1, 2, WANG Xiang( ) 2, LI Xinlin( ) 2, YANG Lei( ) 2 1. School of Materials Science and Engineering, Harbin
More informationSimplified pressure model for quantitative shrinkage porosity prediction in steel castings
IOP Conference Series: Materials Science and Engineering Simplified pressure model for quantitative shrinkage porosity prediction in steel castings To cite this article: A V Catalina and C A Monroe 01
More informationAnalysis of Grain Selection during Directional Solidification of Gas Turbine Blades
Analysis of Grain Selection during Directional Solidification of Gas urbine Blades H. B. Dong Abstract In this paper the evolution of grain structure and the control of crystal orientation in gas turbine
More informationSurface formation in direct chill (DC) casting of 6082 aluminium alloys
IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS Surface formation in direct chill (DC) casting of 682 aluminium alloys To cite this article: N Bayat and T Carlberg 216 IOP Conf.
More informationPresented at the Flemings Symposium, Boston, MA, June 2000 MODELING OF MACROSEGREGATION: PAST, PRESENT AND FUTURE. Christoph Beckermann
Presented at the Flemings Symposium, Boston, MA, June 2000 MODELING OF MACROSEGREGATION: PAST, PRESENT AND FUTURE Christoph Beckermann Department of Mechanical Engineering University of Iowa Iowa City,
More informationDirectional Solidification Microstructure of a NiBased Superalloy: Influence of a Weak Transverse Magnetic Field
Materials 2015, 8, 34283441; doi:10.3390/ma8063428 Article OPEN ACCESS materials ISSN 19961944 www.mdpi.com/journal/materials Directional Solidification Microstructure of a NiBased Superalloy: Influence
More information